Transcript of "numerical analysis of indentation-induced cracking of brittle coatings on ductile substrates"
1.
International Journal of Solids and Structures 39 (2002) 1427–1442 www.elsevier.com/locate/ijsolstr Numerical analysis of indentation-induced cracking of brittle coatings on ductile substrates A. Abdul-Baqi a, E. Van der Giessen b,* a Delft University of Technology, Koiter Institute Delft, Mekelweg 2, 2628 CD Delft, Netherlands b University of Groningen, Department of Applied Physics, Nyenborgh 4, 9747 AG Groningen, Netherlands Received 15 August 2001; received in revised form 7 November 2001Abstract Cracking of hard coatings during indentation is studied using the ﬁnite element method. The coating is assumed tobe linear elastic, the substrate is elastic-perfectly plastic and the indenter is spherical and rigid. Through-thicknesscracks are modeled using cohesive surfaces, with a ﬁnite strength and fracture energy. The interface between the coatingand the substrate is also modeled by means of cohesive zones but with interface properties. The primary potentiallocations for the initiation of coating cracks are the coating surface close to the contact edge and the coating side of theinterface in the contact region, where high values of tensile radial stress are found. Circumferential cracks are found toinitiate from the coating surface and to propagate towards the interface. The initiation and advance of a crack isimprinted on the load–displacement curve as a kink. The spacing between successive cracks is found to be of the orderof the coating thickness. The inﬂuence of other material and cohesive parameters on the initiation of the ﬁrst crack andspacing between successive cracks is also investigated. Ó 2002 Elsevier Science Ltd. All rights reserved.Keywords: Indentation; Fracture; Coatings; Cohesive surface1. Introduction Hard coatings on relatively soft substrates and their industrial applications have been receiving more andmore attention during the past few decades. The coating industry has advanced considerably in the pro-duction of various kinds of coatings to cope with the increasing number of applications of hard-coatedsystems. Hard coatings are usually applied to relatively soft substrates to enhance reliability and perfor-mance. Hard ceramic coatings, for example, are used as protective layers in many mechanical applicationssuch as cutting tools. Such coatings are usually brittle and subject to fracture of the coating or failure of theinterface with the substrate. Therefore, the enhancement gained by the coatings is always accompanied bythe risk of such failure. Indentation is one of the traditional methods to quantify the mechanical properties of materials. Severaltechniques have been reported in the literature to extract the mechanical properties of both homogeneous * Corresponding author. Fax: +31-50-363-4881. E-mail address: giessen@phys.rug.nl (E. Van der Giessen).0020-7683/02/$ - see front matter Ó 2002 Elsevier Science Ltd. All rights reserved.PII: S 0 0 2 0 - 7 6 8 3 ( 0 1 ) 0 0 2 8 0 - 3
2.
1428 A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442and composite or coated materials from indentation experiments (Bhattacharya and Nix, 1988; Doernerand Nix, 1986; Gao et al., 1992; King, 1987; Lim et al., 1999; Oliver and Pharr, 1992). Indentation has alsobeen advocated as a tool to characterize the properties of thin ﬁlms or coatings. At the same time, forexample for hard wear-resistant coatings, indentation can be viewed as an elementary step of concentratedloading. For these reasons, many experimental as well as theoretical studies have been devoted to inden-tation of coated systems during recent years. Contact-induced failure of coated systems has also been investigated during recent years (Abdul-Baqiand Van der Giessen, 2001a,b; Li et al., 1997; Li and Bhushan, 1998; van der Varst and de With, 2001;Malzbender et al., 2000; Wang et al., 1998). The main emphasis in such investigations has been to extractquantitative data about the coating and interfacial fracture energies and strengths. Diverse results havebeen obtained by diﬀerent studies due to the complex nature of the problem and the diﬀerent estimationprocedures (van der Varst and de With, 2001). The complexity is mainly attributed to the fact that suchsystem is a combination of at least two materials with diﬀerent mechanical properties. Failure of suchsystems may include, for example, the plastic deformation of the substrate, the cracking of the coating orthe failure of the interface. Interfacial delamination has been studied by the authors in previous work(Abdul-Baqi and Van der Giessen, 2001a,b). In the absence of coating cracking, delamination was found tooccur in mode II driven by the shear stress at the interface outside the contact region during the loadingstage. During the unloading stage, delamination was found to occur in mode I driven by the tensile stress atthe interface in the contact region. Coating cracking is one of the common failure events usually observed in indentation experiments.Radial or circumferential cracks might initiate from the coating surface or from the coating side of theinterface and may grow into a through-thickness crack. Li et al. (1997) have proposed a method to estimatethe fracture toughness from indentation tests. From the load drop or plateau caused by the ﬁrst circum-ferential crack, they estimate a strain energy release to create the crack. The fracture energy is then cal-culated using the energy release, the crack area and the elastic properties of the coating. This approach hasbeen also used by others (Li and Bhushan, 1998; van der Varst and de With, 2001; Malzbender et al., 2000).van der Varst and de With (2001) have performed Vickers indentation experiments on TiN coatings on toolsteel. Arguing that the energy release which is estimated from the load–displacement curve is spent in bothcreating the crack and some plastic dissipation in the substrate, they estimate an upper bound of 54 J/m2 forthe fracture energy of the coating. However, the method they have used to estimate the energy release fromthe load–displacement curve is diﬀerent from the one suggested by Li et al. (1997). The objective of the present paper is to provide an improved understanding of coating cracking duringindentation. To this end, numerical simulation of the indentation process is performed. The coating isassumed elastic and strong, the substrate is elastic-perfectly plastic and the indenter is spherical and rigid.Coating cracking is modeled by means of cohesive zones. The cohesive zone methodology allows the studyof crack initiation and propagation without any separate criteria since the fracture characteristics of thematerial are embedded in a constitutive model for the cohesive zone. The emphasis in this study will be oncircumferential cracks which initiate from the coating surface, its imprint on the load–displacement curveand the spacing between successive cracks. Using our numerical ﬁndings, the above-mentioned estimatesof the fracture energy are tested. The eﬀect of the material, geometric and cohesive parameters is alsoinvestigated.2. Problem formulation The system considered in this study is illustrated in Fig. 1. It comprises an elastic-perfectly plasticsubstrate coated by an elastic thin coating and indented by a spherical indenter. The indenter is assumedrigid and only characterized by its radius R ¼ 25 lm. Assuming both coating and substrate to be isotropic,
3.
A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442 1429Fig. 1. Geometry of the analyzed problem, including deﬁnition of local frame of reference, ðq; fÞ, and detail of the layout of continuumelements and cohesive elements along the interface.the problem is axisymmetric, with radial coordinate r and axial coordinate z in the indentation direction.The coating is characterized by its thickness t ¼ 1 lm and elastic properties (Ec ¼ 500 GPa, mc ¼ 0:33) andis bonded to the substrate by an interface. The substrate is supposed to be a standard isotropic elastoplasticmaterial with plastic ﬂow being controlled by the von Mises eﬀective stress re . It is taken to have a heightL À t and a radius L, with L large enough compared to ﬁlm thickness so that the solution is independent ofL and the substrate can be regarded as a half space; thus, it is only characterized by its elastic properties(Es ¼ 200 GPa, ms ¼ 0:33) and the yield stress ry ¼ 1:0 GPa. The precise boundary conditions are also illustrated in Fig. 1. The indentation process is performed _incrementally with a constant indentation rate h ¼ 1 mm/s. Outside the contact area, with radius a mea-sured in the reference conﬁguration, the ﬁlm surface is traction free, tr ðr; 0Þ ¼ tz ðr; 0Þ ¼ 0 for a 6 r 6 L: ð1Þ Inside the contact area we assume perfect sliding conditions. The boundary conditions are speciﬁed withrespect to a local frame of reference ðq; fÞ that is rotated over an angle / such that f is always perpendicularto the coating surface as shown in Fig. 1. The deﬁnition of this frame for points inside the material is alsoshown in Fig. 1. The angle / is calculated for each material element in the deformed state (solid line) basedon the rotation of the element with respect to its original conﬁguration (dashed line). In the normal di-rection, the displacement rate uf is controlled by the motion of the indenter, while in the tangential direction _the traction tq is set to zero, i.e. _ _ uf ðr; zÞ ¼ h cos /; tq ðr; zÞ ¼ 0 for 0 6 r 6 a: ð2ÞThe substrate is simply supported at the bottom, so that the remaining boundary conditions read uz ðr; LÞ ¼ 0 for 0 6 r 6 L; ur ð0; zÞ ¼ 0 for 0 6 z 6 L: ð3ÞThe indentation force F is computed from the tractions in the contact region, Z a F ¼ tz ðr; 0Þ2pr dr: ð4Þ 0 The analysis is carried out numerically using a ﬁnite strain, ﬁnite element method. The mesh is anarrangement of four-noded quadrilateral elements. The elements are built up of four linear strain triangles
4.
1430 A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442in a cross arrangement to minimize numerical problems due to plastic incompressibility. To resolveproperly the high stress gradients under the indenter and for an accurate detection of the contact nodes, themesh is made very ﬁne locally near the contact area with an element size of t=10. Since the indenter is rigid, contact nodes are identiﬁed simply by their spatial location with respect to theindenter. At a certain indentation depth h and displacement increment Dh, the node is considered to be incontact if the vertical distance between the node and the indenter is not greater than Dh. Local loss ofcontact may occur if an open crack falls into the contact region. In the calculations, contact is releasedwhen the nodal force becomes tensile. We have used a threshold value for tensile nodal forces equal to theaverage current nodal force. A value that is an order of magnitude smaller did not show any signiﬁcanteﬀect on the results. After a node is released from contact, the distance between the node and the indenter ischecked each increment for possible re-formation of contact. Coating cracking is represented by inserting cohesive zones into the coating, perpendicular to the sur-face. A cohesive zone is also used to model the interface between coating and substrate. A cohesive zone is asurface along which a small displacement jump between the two sides is allowed with normal and tangentialcomponents Dn and Dt , respectively. The cohesive behavior is speciﬁed in terms of a constitutive equationfor the corresponding traction components Tn and Tt at the same location. The cohesive law we adopt in this study is the one given by Xu and Needleman (1993). The tractioncomponents are determined by two potentials /n ðDn ; Dt Þ and /t ðDn ; Dt Þ according to o/n o/t Tn ¼ ; Tt ¼ : ð5Þ oDn oDtThe resulting traction-separation relations in normal and tangential direction are illustrated in Fig. 2. Inboth directions, the peak traction represents the cohesive strength and the area under the curve correspondsto the work of fracture. The work of normal (tangential) separation, /n (/t ), can be expressed in terms ofthe corresponding strengths rmax (smax ) as rﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ 1 /n ¼ expð1Þrmax dn ; /t ¼ expð1Þsmax dt ; ð6Þ 2where dn and dt are two characteristics lengths and q ¼ /t =/n is a coupling parameter. From the previousequations, the normal and tangential strengths are related byFig. 2. The normal and shear cohesive tractions: (a) normal traction Tn ðDn Þ and (b) shear traction Tt ðDt Þ. Both are normalized by theirrespective peak values rmax and smax .
5.
A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442 1431 1 dt rmax ¼ pﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ smax : ð7Þ q 2 expð1Þ dnMore details of this constitutive model are found in Xu and Needleman (1993) and Abdul-Baqi and Vander Giessen (2001a). The cohesive zones are incorporated in the ﬁnite element calculation using linear twonoded elements with two Gaussian integration points which is consistent with the type of continuum el-ements in the coating and the substrate. For the cohesive zones at the interface we have chosen dn ¼ dt ¼ 0:1 lm, q ¼ 0:4288 and /n ¼ 200 J/m2 . iMaking use of Eqs. (6) and (7), these values correspond to rimax ¼ smax ¼ 7:36 GPa. For the coating dn ¼dt ¼ 1:0 nm, q ¼ 0:4288 and /n ¼ 30 J/m2 so that rc ¼ sc ¼ 11 GPa. The values assigned to the work of max maxseparation for both coating and interface are comparable to these obtained by Wang et al. (1998) for di-amond-like carbon coatings on steel substrates. The values assigned to the characteristic lengths dn and dtfor both interface and coating were chosen such that, when combined with the work of separation, rea-sonable values for the strength are obtained. In terms of the coating material and the cohesive parameters,the critical stress intensity factors for mode I and II fracture along a cohesive zone, i.e KIC and KIIC , are 2 1=2 2 1=2ðEc /n =ð1 À mc ÞÞ and ðEc /t =ð1 À mc ÞÞ , respectively (Xu and Needleman, 1994). The ratio of KIIC to KIC pﬃﬃﬃbeing q is about 0.65. This value is reasonable compared to the values obtained by diﬀerent experimentalestimates as listed in Malzbender et al. (2000). The eﬀect of the variation of some of previously given parameters, such as the coating thickness, thecoating Young’s modulus, the yield stress and the coating cohesive parameters will be investigated. Thevalues given in this section will serve as a reference case in this study. In the remainder of this study we willdrop the superscripts from quantities referring to the cohesive parameters since, unless otherwise speciﬁed,they all will refer to the coating.3. Stress distribution in a perfect coating Before performing the cracking analysis, it is instructive to have a brief look at the stresses that generatein a perfect coating during indentation (i.e. without cohesive zones). Fig. 3(a) shows the radial stress dis-tribution along the coating surface, rqq ðrÞ. A tensile radial stress is found outside the contact area with amaximum at r % 1:25a, where a is the instantaneous contact radius. It should be noted that the location ofthis maximum is strongly dependent on the ratio t=R. For the same indentation depth, the smaller the ratiot=R, the closer the location of the maximum tensile stress to the contact edge. The radial stress is found to becompressive within the contact area r < a. It is interesting to note in Fig. 3(a) the decrease of the com-pressive stress in the contact region with increasing indentation depth. This is a consequence of the plasticﬂow of the substrate material in the indented region which induces an additional positive radial straining inthe coating, leading to a decrease in the compressive stress at the contact region. Tensile stress is also seenalong the coating side of the interface as shown in Fig. 3(b). It is located at the contact region r < a with amaximum at the symmetry axis. This suggests that a circumferential crack is likely to initiate from theinterface at r < a or the coating surface at r % 1:25a due to the maximum tensile radial stresses at theseregions. The distribution of the shear stress rqf along the mid-plane of the coating is shown in Fig. 3(c). Thehighest value of this stress is found under the contact edge at r ¼ a. The shear stress has a smaller maximumvalue than the radial stress and furthermore is located at the edge of the contact where only relatively smalltensile radial stresses are found. This indicates that shear stress is likely to play a minor role in the fractureprocess. Comparing the radial stresses along the surface with those on the coating side of the interface, wesee that each tensile stress is faced by a compressive stress on the opposite side of the coating due to thebending-like loading. This indicates that a crack, whether initiated at the surface or the interface, will not be
6.
1432 A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442Fig. 3. Stress distribution at several indentation depths for t=R ¼ 1=25: (a) radial stress along the coating surface, (b) radial stress alongthe coating side of the interface and (c) shear stress along the middle plane in the coating (z ¼ t=2).able to propagate through the whole coating thickness. Tensile radial stresses at the surface and interfaceare seen to be of the same order of magnitude. But crack initiation and propagation from the coating side ofthe interface suﬀers an extra resistance as this requires some interfacial shearing (see inset in Fig. 1) andhence more energy. Therefore, the main emphasis in this study will be on cracks that initiate from thecoating surface and advance towards the interface. Cracks which initiate from the coating side of the in-terface do not have any signiﬁcant eﬀect on surface cracks as will be discussed later in this paper.4. Analysis A ﬁrst approach to simulate coating failure was to place cohesive zones in between all continuum ele-ments in the coating, as pioneered by Xu and Needleman (1993, 1994). Contrary to their work, however,the present computation is a quasi-static one and this led to serious numerical problems. The numericalproblems originate from the fact that some adjacent cohesive zones reach the peak traction rmax and startsoftening almost simultaneously, which breaks the uniqueness of the solution. Mesh reﬁnement does not
7.
A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442 1433solve the problem. When ﬁne meshes are used, the region of more or less homogeneous, high tensile radialstresses comprises several elements so that there is an even larger probability of running into a loss ofuniqueness. On the other hand, using coarser meshes to overcome this problem decreases the accuracy inrepresenting the high stress gradients in the coating and the precise contact between the indenter and thecoating. In addition, embedding of cohesive elements leads to an artiﬁcial enhancement of the overallcompliance (Xu and Needleman, 1994). This increase will tend to underestimate the stresses in the coatingand therefore the occurrence of failure. Since the compliance increase is proportional to the number ofcohesive zones, we adopt a procedure in this study in which the number of cohesive zones is minimized. The location of the necessary cohesive zones is determined in the following way. We ﬁrst conduct acalculation without any cohesive zone and we trace the evolution of the maximum tensile radial stress alongthe coating surface along with its location at each indentation increment. This is shown in Fig. 4, with thesteps in the curves originating from the node-to-node growth of the contact region. After an initial tran-sient, both the maximum stress and its location seem to increase linearly with the contact radius a. The ﬁrstcrack is predicted to occur when rmax ¼ rmax . Fig. 4 shows that rmax ¼ 11 GPa is reached when the contact qqradius a is 3:7 lm (h ¼ 0:5 lm) and at the radial location r ¼ 5:0 lm. In the second step, a new calculation is carried out with a single cohesive zone being placed at thislocation prior to indentation. The ﬁrst crack will then indeed form at the expected indentation depth and wecontinue the computation to determine the location of the second crack in the same way as for the ﬁrstcrack. A third computation is then started with two cohesive zones, etc. Continuing this procedure, morecracks are simulated. Fig. 5 gives the result after the fourth step in which three coating cracks have de-veloped. Fig. 5(a) shows the distribution of radial stress rqq at an indentation depth of 0.75 lm. The ﬁrstcrack at r ¼ 5:0 lm is visible in the ﬁgure and a tensile stress is seen to develop in the coating outside thecrack radius. At an indentation depth of h ¼ 1:25 lm, three cracks have already occurred at locations 5.0,6.4 and 7.9 lm, see Fig. 5(b). The crack at r ¼ 6:4 lm is not visible in the ﬁgure since it has closed up. Theﬁrst crack has also closed from the surface side as a result of the compressive stress in the contact region.Note that local loss of contact has occurred above the closed-up crack as explained in Section 2. The thirdcrack did not reach the interface yet at this stage of loading due to the compressive stress in this region. The procedure is further illustrated in Fig. 6(a), showing the evolution of the maximum radial stressalong the coating surface. The maximum stress is seen to increase with indentation depth until the momentFig. 4. (a) Evolution of the maximum radial stress at the coating surface rmax with the contact radius a and (b) the corresponding qqlocation r at the coating surface at which the stress is maximum.
8.
1434 A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442 Fig. 5. Distribution of the radial stress rqq at indentation depths of 0.75 lm (a) and 1.25 lm (b).Fig. 6. (a) Evolution of the maximum radial stress at the coating surface rmax with the indentation depth h. The curves belong to four qqdiﬀerent calculations with the number of cohesive surfaces (and later cracks) increasing from 0 to 3. (b) Load–displacement curve forthe case shown in Fig. 5. Arrows point to sudden load drops caused by cracking events.of failure where a sudden drop occurs due to stress relaxation and redistribution. After initiation, the crackpropagates through the coating thickness and stops just before reaching the interface due to the com-pressive stress at that region. About 10% of the coating thickness remains intact for a while until it shearsoﬀ (mode II) and later opens in mode I resulting in two small drops in the maximum stress. The location ofthe fourth crack is predicted to be r ¼ 9:4 lm after h ¼ 1:55 lm. The four successive cracks thus found areseen to have an almost uniform spacing k of 1:5 lm. The dependence of crack spacing on some of the modelparameters will be discussed in Section 5. The corresponding load–displacement curve shown in Fig. 6(b) reﬂects these cracking events by a suddendrop of the load. Each of three major drops on the curve is associated with the initiation of a crack. Sincethe fracture energy is proportional to the crack radius, the larger the crack radius, the larger the drop in theload. With further indentation, the contact radius increases, thus expanding the tensile region at the in-terface. The growth of the freshly nucleated crack to the interface gives rise to small load drops in betweenthe major ones. The third crack shown in Fig. 5(b) for example reaches the interface forming a completethrough-thickness crack at an indentation depth of 1.3 lm. This gives rise to the small load drop seen on theload–displacement curve at this depth.
9.
A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442 1435 These results demonstrate that the procedure described above is indeed capable of predicting the initi-ation and growth of coating cracks within the cohesive zone framework. It should be pointed out, however,that even with this small number of cohesive zones, some numerical problems were faced at ﬁrst. Carefulexamination has shown that these were caused by the fact that the cohesive zone parameters chosen hereapproach atomic separation properties. The coating strength is on the order of tens of GPa’s and the criticalopening is only a nanometer. The consequence of this is that the cohesive stiﬀness beyond the peak strengthis very large, and negative, which would lead to local snap back in the ﬁnite element system. This canprobably be dealt with using, for instance, indirect displacement control (de Borst, 1987), but we haveadopted a simpler method to circumvent this. The idea is to reduce the instantaneous stiﬀness of the co-hesive zone as soon as the normal strength is reached, Dn P dn , but to update the tractions directly from Eq.(5). Of course, this leads to an error in the solution, but this error is corrected by way of the equilibriumcorrection in the next time step. Practically speaking, the eﬀect of this procedure is that snap back insta-bilities are avoided and stability is maintained. Extensive testing has shown that the ﬁnal error in, forexample, the traction continuity between a cohesive zone element and a continuum element is smaller thana few percent, even when the instantaneous cohesive zone stiﬀness is reduced down to 5%. Cracks initiating from the coating side of the interface have been excluded from the simulations despitethe high tensile stress found there. The main reason is the fact that the maximum tensile stress is alwaysfound at the symmetry axis (Fig. 3b). A cohesive surface at this location will have a zero area in an axi-symmetric formulation making it impossible to simulate. To study the eﬀect of coating cracking startingfrom the interface, three cohesive surfaces are placed at radial locations of 1.5, 3.0 and 4.5 lm. Being alllocated at distances less than 5.0 lm (the expected location of the ﬁrst surface crack), surface cracks are notexpected to occur. The radial stress distribution at an indentation depth of 1.0 lm and the evolution of themaximum radial stress on the coating surface are shown in Fig. 7. Cracks at the three speciﬁed locations areseen to have occurred. None of these cracks has reached the surface since at the moment of initiation ofeach crack, the opposite side of the coating is already in contact and hence the stress state is compressive.The stress at the coating surface outside the contact region is mainly driven by the contact between theindenter and the coating at the contact edge r ¼ a. Since all cracks initiating from the coating side of theinterface lie in the region r < a, their eﬀect on the stress outside the contact region is insigniﬁcant as shownin Fig. 7(b).Fig. 7. (a) Distribution of the radial stress rqq at an indentation depth of 1.0 lm. It illustrates the three cracks initiating from thecoating side of the interface at locations 1.5, 3.0 and 4.5 lm. (b) The corresponding maximum radial stress at the coating surface rmax qq(solid line) compared with the stress of the noncracked coating (dashed line).
10.
1436 A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–14425. Eﬀect of geometrical, material and cohesive parameters The eﬀect of various parameters on the initiation of the ﬁrst circumferential crack and the spacing kbetween successive cracks is studied. The chosen parameters are: the coating thickness t, the coatingYoung’s modulus Ec , the substrate yield stress ry and the cohesive properties, i.e. coating strength rmaxas well as the coupling and reversibility of the cohesive tractions. The coating thickness t and indenter radius R are the main length scales in the system and their eﬀect isstudied by varying the nondimensional parameter t=R. Fig. 8 shows the variation of the crack spacingwith the coating thickness. The relation k=R % 1:4t=R provides the best linear ﬁt. It should be noted thatspacing in this ﬁgure is taken to be distance between the ﬁrst two cracks. From the average spacing we getk=R % 1:5t=R. In the remainder of this study, k will refer to the average crack spacing. Fig. 9 shows the location of the ﬁrst crack as a function of the coating thickness and correspondingindentation depth for two values of rmax . It can be seen that ﬁrst crack occurs closer to the contact edge forFig. 8. Normalized crack spacing ðk=RÞ versus normalized coating thickness ðt=RÞ. Single points are the numerical results and solid lineis a linear ﬁt. The error in k is ðÆÞ half the ﬁnite-element size.Fig. 9. The location of the ﬁrst circumferential crack as a function of the coating thickness (a) and the corresponding indentation depth(b) for two values of rmax . Discrete points are numerical results, lines are linear ﬁts.
11.
A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442 1437thinner coatings and higher strengths. Moreover, the thicker the coating the larger the indentation depthrequired to form the ﬁrst crack. A variation of the coating’s Young’s modulus Ec ranging from 200 to 500 GPa did not have any eﬀect oncrack spacing. However, the location of the ﬁrst crack and the corresponding indentation depth stronglydepend on Ec . The radial stress in the coating rqq is proportional to the degree of bending and to Young’smodulus. Therefore, coatings of lower modulus require more bending or equivalently larger indentationdepths to reach the fracture strength and subsequently crack. Since the location of the maximum stress onthe coating surface increases with indentation depth (Fig. 4b), coatings of lower Young’s modulus crack atlarger radii as seen in Fig. 10. An increase in the coating strength rmax seems to be equivalent to a decreasein the Young’s modulus in terms of location of the ﬁrst crack and the corresponding indentation depth asshown in Fig. 10. This suggests that the ﬁrst crack radius and the corresponding indentation depth dependon the ratio rmax =Ec which can be considered a measure of the critical strain for cracking. Contrary to theYoung’s modulus, the coating strength does have some inﬂuence on crack spacing. Strengths of rmax ¼ 5:5and 16:5 GPa resulted in crack spacings of 1.2 and 1.8 lm, respectively. The eﬀect of the yield stress ry of the substrate is studied by comparing the results obtained using threediﬀerent values, namely, 0.5, 1.0 and 2.0 GPa. These values resulted in ﬁrst circumferential cracks of radii of5.6, 5.0 and 4.7 lm, respectively. The corresponding indentation depths did not deviate signiﬁcantly fromthe reference case, where h ¼ 0:5 lm. The crack spacing increased to 1.9 lm for ry ¼ 0:5 GPa, whereas itdecreased to 1.2 lm in the case of ry ¼ 2:0 GPa. The eﬀect of the yield stress is explained in terms of the sizeof the plastic zone. At the same indentation depth h, the lower the yield stress, the larger the plastic zonesize. The expansion of the plastic zone towards the surface is partially accommodated by bending of thecoating outside the contact region. Therefore, lower yield stresses tend to lead to larger radial location ofthe maximum stress on the coating surface and therefore a larger crack radius. The corresponding largercrack spacing is also explained by the same argument. The eﬀect of friction between the indenter and the coating on the location of the ﬁrst crack and the crackspacing is also investigated. In the case of perfect sticking contact conditions, the ﬁrst crack occurred ata radius r ¼ 5:5 lm and a corresponding indentation depth h ¼ 0:59 lm, instead of r ¼ 5:0 lm andFig. 10. The location of the ﬁrst circumferential crack versus the corresponding indentation depth. Open circles are the numericalresults using Ec of 200, 300, 400 and 500 GPa, rmax ¼ 11 GPa. Stars correspond to values of rmax of 5.5, 8.25, 11 and 16:5 GPa,Ec ¼ 500 GPa. Lines are quadratic ﬁts.
12.
1438 A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442h ¼ 0:5 lm obtained previously in the case of perfect sliding contact. The crack spacing also increased from1.5 to 2 lm when perfect sticking was assumed. Souza et al. (2001) have experimentally investigated the spacing of indentation-induced cracks in tita-nium nitride coatings on stainless steel substrates. They have used a Rockwell B indenter (R ¼ 795 lm) andcoating thicknesses of 0.4, 2.1 and 4.2 lm. They have found that cracks are almost uniformly spaced whichis consistent with our numerical results. The crack spacings observed for the various thicknesses were foundto be 1.5, 5.0 and 10.0 lm, respectively, so that k=R varies between 2:4t=R and 3:75t=R. However, theseexperimental values are seen to be larger than those obtained in our calculations. There may be severalreasons for this discrepancy. One reason is the presence of residual compressive stresses of 0.7–1.5 GPa inthe coatings investigated by Souza et al. (2001), whereas in the current simulations, the coating is assumedto be stress free prior to indentation. Another reason is the friction between the indenter and the coatingwhich is usually present in indentation experiments. In the presence friction, the crack spacing increases asmentioned previously. In addition, the material parameters chosen in this study are not precisely those oftitanium nitride coatings on stainless steel substrates. Variation of these parameters has been shown aboveto inﬂuence the crack spacing. The coupling and reversibility in the cohesive law are also investigated. In the original Xu-Needlemanformulation (Xu and Needleman, 1993), the constitutive law of the cohesive zone is assumed to be re-versible, so that the loading and unloading paths are the same. In this case, if a crack closes it heals and thesystem recovers all the energy consumed. Even though this energy is very small in comparison withthe plastic dissipation, the eﬀect of taking it into account is studied by using an irreversible version of thetractions. Therefore, we modify the constitutive law by introducing a secant unloading branch as illustratedin Fig. 11. If the opening velocity changes sign (unloading), the traction is assumed to decrease linearly tozero as the opening diminishes to zero (Camacho and Ortiz, 1996). The same method is applied to the sheartraction. It should be noted that in the presence of coupling between the tractions, the formulation forirreversibility would not be clear. Therefore, the eﬀect of reversibility is studied by comparing the resultsachieved when using reversible and irreversible uncoupled tractions. On the other hand, the eﬀect ofcoupling is investigated by studying the diﬀerence between using coupled and uncoupled reversible trac-tions. The results of coupled reversible tractions which has been used so far are compared to the resultsobtained when using uncoupled reversible tractions; i.e., Tn ¼ Tn ðDn ; Dt ¼ 0Þ and Tt ¼ Tt ðDt ; Dn ¼ 0Þ (cf. Fig. 11. Irreversible normal cohesive traction Tn ðDn Þ at Dt ¼ 0.
13.
A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442 1439 Fig. 12. Load–displacement curve for uncoupled traction-separation laws in the cohesive zones compared to the coupled ones.Fig. 2). Three cracks were simulated and the location of the fourth one is predicted as explained in Section4. The crack spacing is found to be 1.3 lm, which is less than the value of 1.5 lm found previously inthe presence of coupling. Moreover, additional cracks occur at smaller indentation depths compared to thecorresponding ones in the presence of coupling. This is demonstrated in Fig. 12. When a crack opens, theshear strength is reduced in the presence of coupling as demonstrated in Fig. 2(b). The moment the crackreaches the interface, it shears oﬀ by the shear stress which is present around the contact edge (Fig. 3c). Theshearing leads to some relaxation of the coating in the form of unbending. Compared to the uncoupledtractions where shearing oﬀ does not occur, indenting to larger depth is required to arrive to the samedegree of bending and form an additional crack. Moreover, larger indentation depth means that themaximum tensile stress on the coating surface occurs at a larger radius. This explains the larger crackspacing in the case of coupling. Reversibility of the tractions does not seem to have any signiﬁcant eﬀect onthe results, even though we have noticed crack closure taking place (e.g. Fig. 5b). Uncoupled reversible andirreversible tractions lead to almost indistinguishable load–displacement curves and to the same crackspacing, k ¼ 1:3 lm.6. Fracture energy estimates Several researchers have tried to estimate the fracture energy from indentation experiments. One of theapproaches which has been used is to estimate the energy consumed to create the ﬁrst circumferential crackfrom the corresponding load drop or plateau on the load–displacement curve (Li et al., 1997; Li andBhushan, 1998; van der Varst and de With, 2001; Malzbender et al., 2000). In this section we will comparethe prediction of these methods with our numerical ﬁndings. Li et al. (1997) have suggested an approach which is based on the idea that all the energy released uponthe formation of a crack, DU , is consumed in creating the crack with fracture energy /n per unit area. Bydetermining DU , the fracture energy can be estimated as est DU /n ¼ ; ð8Þ 2prtwith r the crack radius and t the coating thickness. Two methods have been suggested in the literature toestimate DU from the load–displacement curve, as illustrated in Fig. 13. The ﬁrst method (Li et al., 1997) is
14.
1440 A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442Fig. 13. Schematic load–displacement curve. DU1 to DU3 are diﬀerent estimates of the energy release associated with a cracking event.Fig. 14. Estimates for /n from Eq. (8). /est1 , /est2 and /est3 are based on the energies DU1 , DU2 and DU3 (cf. Fig. 13), respectively. (a) n n nEstimated values versus the actual ones for t ¼ 1:0 lm. (b) Estimated values versus the coating thickness for /n ¼ 30 J/m2 . In (a) and(b) single points are numerical results and lines are linear ﬁts.to extrapolate the load in a tangential direction from the beginning to the end of the discontinuity. Thediﬀerence between the areas under the extrapolated curve and the discontinuous one (DU1 in Fig. 13) istaken to be the estimate of the energy release. The second method (van der Varst and de With, 2001) es-timates the energy release as half the cracking load Fc times the displacement jump Dh (DU2 in Fig. 13).We here suggest a third method which estimates the energy release as half the cracking indentation depthhc times the load jump (DU3 in Fig. 13). The second and third methods are borrowed from linear elasticfracture mechanics for cracking under constant load and constant displacement (indentation depth), re-spectively (Kanninen and Popelar, 1985). We now use our numerical simulations to test the accuracy of the estimates obtained from Eq. (8).Obviously, the values of the energy release estimated in the three methods are completely diﬀerent and sowill be the estimated fracture energies. Based on our numerical results, Fig. 14 shows the estimated valuesof the coating fracture energy for several values of /n and t. At low values of /n or t, the ﬁrst methodunderestimates the fracture energy, whereas the second and third methods give reasonable estimates. On theother hand, at large values of /n or t, the second and third methods overestimate the fracture energy,
15.
A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442 1441whereas the estimation by the ﬁrst method seems reasonable. Therefore, estimations of the coating fractureenergy from indentation experiments might lead to values diﬀerent from the actual ones by as much as oneorder of magnitude. The origin for the discrepancy is the fact that the estimates assume linearity of theproblem, while in fact it is quite nonlinear because of the energy dissipation in the plastic zone in thesubstrate. Nevertheless, it is interesting to note the proportionality between the normalized estimated valuesand the actual ones and the coating thickness.7. Concluding remarks In this paper, cracking of hard coatings on elastic-perfectly plastic substrates during indentation hasbeen studied using the ﬁnite element method. Cracking of the coating was simulated by assuming single ormultiple planes of potential cracks across the coating thickness at pre-determined radial locations priorto indentation. These planes are assigned a ﬁnite strength and modeled by means of cohesive zones. Theinterface between the coating and the substrate was also modeled by means of cohesive zones but withinterface properties. The emphasis was on circumferential cracks which initiate from the coating surface outside the contactedge and advance towards the interface. The initiation and advance of such cracks is imprinted on the load–displacement curve as a sudden load drop (kink). The larger the crack radius, the larger the load drop, sincethe energy released by the crack is proportional to the crack area. After initiation, the crack advances almostspontaneously across the coating thickness and stops just before reaching the interface as a result of acompressive stress at that side. With further indentation, the tensile region under the indenter expands andwhen it encompasses the crack tip, the crack advances until the interface creating a complete through-thickness crack. This is also imprinted on the load–displacement curve by a relatively smaller load drop. Forseveral coating thicknesses, the ratio of the crack radius to the instantaneous contact radius was found toincrease linearly with the coating thickness. The smaller the coating thickness, the closer this ratio is to unity. With further indentation, successive cracking occurs at larger radii, which each additional crack alsoimprinted on the load–displacement curve as a kink. The crack spacing was found to be predominantlycontrolled by the ratio of the coating thickness to the indenter radius. For a ﬁxed indenter radius, the crackspacing is of the order of the coating thickness. Variation of the coating Young’s modulus did not show anyinﬂuence on crack spacing, whereas spacing increased with the coating strength and decreased with thesubstrate yield stress. Coupling and irreversibility of the cohesive tractions were also investigated. Thepresence of coupling was found to slightly increase crack spacing. Moreover, additional cracking occurs athigher indentation depths compared to uncoupled tractions. Reversible and irreversible cohesive tractionshave led to almost indistinguishable results in terms of crack spacing and load–displacement data. Thepredicted crack spacings are consistent with those obtained in recent experiments by Souza et al. (2001). Finally, it has been shown that estimation of the coating fracture energy from the ﬁrst crack area andcorresponding load drop, as commonly done in indentation experiments, leads to values diﬀerent from theactual ones by as much as one order of magnitude. The reason for this is that a small portion of the energyrelease is consumed by the crack, while the rest of the energy is consumed by the accompanied plasticdissipation in the substrate.ReferencesAbdul-Baqi, A., Van der Giessen, E., 2001a. Indentation-induced interface delamination of a strong ﬁlm on a ductile substrate. Thin Solid Films 381, 143–154.Abdul-Baqi, A., Van der Giessen, E., 2001b. Delamination of a strong ﬁlm from a ductile substrate during indentation unloading. J. Mater. Res. 16, 1396–1407.
16.
1442 A. Abdul-Baqi, E. Van der Giessen / International Journal of Solids and Structures 39 (2002) 1427–1442Bhattacharya, A.K., Nix, W.D., 1988. Analysis of elastic and plastic deformation associated with indentation testing of thin ﬁlms on substrates. Int. J. Solids Struct. 24, 1287–1298.Camacho, G.T., Ortiz, M., 1996. Computational modelling of impact damage in brittle materials. Int. J. Solids Struct. 33, 2899–2938.de Borst, R., 1987. Computation of post-bifurcation and post-failure behaviour of strain-softening solids. Comput. Struct. 25, 211–224.Doerner, M., Nix, W., 1986. A method for interpreting the data from depth-sensing indentation instruments. J. Mater. Res. 1, 601–609.Gao, H., Chiu, C.-H., Lee, J., 1992. Elastic contact versus indentation modeling of multi-layered materials. Int. J. Solids Struct. 29, 2471–2492.Kanninen, M.F., Popelar, C.H., 1985. Advanced Fracture Mechanics. Oxford University Press, New York.King, R.B., 1987. Elastic analysis of some punch problems for a layered medium. Int. J. Solids Struct. 23, 1657–1664.Li, X., Bhushan, B., 1998. Measurement of fracture toughness of ultra-thin amorphous carbon ﬁlms. Thin Solid Films 315, 214–221.Li, X., Diao, D., Bhushan, B., 1997. Fracture mechanisms of thin amorphous carbon ﬁlms in nanoindentation. Acta Mater. 45, 4453–4461.Lim, Y.Y., Chaudhri, M.M., Enomoto, Y., 1999. Accurate determination of the mechanical properties of thin aluminum ﬁlms deposited on sapphire ﬂats using nanoindentations. J. Mater. Res. 14, 2314–2327.Malzbender, J., de With, G., den Toonder, J.M.J., 2000. Elastic modulus, indentation pressure and fracture toughness of hybrid coatings on glass. Thin Solid Films 366, 139–149.Oliver, W.C., Pharr, G.M., 1992. An improved technique for determining hardness and elastic modulus using load and displacement sensing indentation experiments. J. Mater. Res. 7, 1564–1583.Souza, R.M., Sinatora, A., Mustoe, G.G.W., Moore, J.J., 2001. Numerical and experimental study of the circular cracks observed at the contact edges of the indentations of coated systems with soft substrates. Wear 251, 1337–1346.van der Varst, P.G.Th., de With, G., 2001. Energy base approach to the failure of brittle coatings on metallic substrates. Thin Solid Films 384, 85–89.Wang, J.S., Sugimura, Y., Evans, A.G., Tredway, W.K., 1998. The mechanical performance of DLC ﬁlms on steel substrate. Thin Solid Films 325, 163–174.Xu, X.-P., Needleman, A., 1993. Void nucleation by inclusion debonding in a crystal matrix. Model. Simul. Mater. Sci. Eng. 1, 111–132.Xu, X.-P., Needleman, A., 1994. Numerical simulations of fast crack growth in brittle solids. J. Mech. Phys. Solids 42, 1397–1434.
Be the first to comment